• Palygorskite • morphology • nanocomposite • rheology • Polypropylene Information on the article: received: March 2014, reevaluated: June 2014, accepted: February 2015
Influence of Chemically Treated Palygorskite Over the Rheological
Behavior of Polypropylene Nanocomposites
Influencia de paligorskita químicamente tratada sobre el comportamiento
reológico de nanomateriales compuestos de polipropileno
Soberanis-Monforte Genaro Antonio
Unidad de Materiales
Centro de Investigación Científica de Yucatán, AC E-mail: firstname.lastname@example.org
Gordillo-Rubio José Luis
Unidad de Materiales
Centro de Investigación Científica de Yucatán, AC E-mail: email@example.com
González-Chi Pedro Iván
Unidad de Materiales
Centro de Investigación Científica de Yucatán, AC E- mail: firstname.lastname@example.org
Autor para correspondencia
Melt compounding was used to prepare thermoplastic composites reinfor-ced with palygorskite; the chemical modification of the palygorskite surface and the control of extrusion parameters were used to promote good disper-sion and a good interface with the matrix, affecting the rheological proper -ties of the mixture, since the melt viscoelastic behavior is sensitive to changes in the molecular structures at nanoscale and mesoscale. The palygorskite nanoclay (diameter 30 nm) was extracted from a site in the southeast of the state of Yucatan, Mexico; the palygorskite was subjected to purification and then superficially modified with 3-aminopropyltrimetoxysilane. These pro -cesses generated three types of specimens: unpurified, purified and puri -fied-silanized palygorskite; which were subsequently incorporated (0.5 w%) to a polypropylene matrix by twin extrusion. Frequency sweeps were used to evaluate the interaction between the matrix and the nano-reinforcement. The master curves of storage modulus (G’), loss modulus (G”) and complex viscosity (η*) vs angular frequency (ωx) show a change of the interfacial
The basic structure of fibrous palygorskite was propo -sed by Bradley in 1940: [Si8Mg5O20(OH)2](H2O)4▪4H2O;
the water molecules associated with the palygorskite structure show three different linkages: hygroscopic water, coordinated water and structural water. Palygorskite is widely used in different applications such as animal waste adsorbent, pesticide carrier, deco-lorizing agent, catalyst and catalyst support and as ex -cipient for medical drugs (Dos Santos, 2013).
The adsorbent and catalytic applications of the palygorskite depend from the surface physico-chemical properties, which can be modified by chemical and thermal treatments to control the surface activity (Jime-nez et al., 1978; Bonilla et al., 1981; Pesquera et al., 1992; Duan et al., 2011). Although palygorskite has been stu-died from different points of view (Abdul & Weaver, 1969; Corma et al., 1987 y 1990; Gonzalez et al., 1990), the literature concerning this mineral is less abundant than that for sepiolite or other smectites.
Clays are being used to create new materials with unique characteristics, and among the most interesting are the composites in which the clay is mixed at nano level with a polymer; these materials are known as po-lymer-silicate nanocomposites (PSNs). They only incorpo-rate a small amount of silicates but provide good mechanical, thermal, and barrier properties (Kojima et al., 1993; Furuichi et al., 1996; Wang et al., 2001; Koo et al., 2005). One of the real challenges posed by the PSNs is the distribution of nano-reinforcement in the matrix, which may affect the range of applications for PSNs
(Chen etal., 2010). Depending on the chemical nature of the constituents and the interactions between nanorein-forcing particles, their dispersion can generate agglo-merated, intercalated and exfoliated structures (Koo et al., 2003).
Molten compounding to disperse the nanoclay in a thermoplastic polymer is a promising technique for manufacturing PSNs, due to its ease of operation (Chen
etal., 2010), low cost and minimal impact on the envi-ronment. This processing method is based on conven-tional polymer blending by twin screw extrusion. When this processing method is used with non-polar poly-mers such as polypropylene (PP), compatibilizing agents are required because the shear stresses generated du -ring the processing are not sufficient to disperse the na -noclay in the matrix. A generally accepted practice is to add maleatedpolypropylene (MaPP) as a compatibilizer. However, parameters like the molecular weight of the MaPP and the content of grafted maleic anhydride (MA) must be taken into account. It has been found that in the case of laminar clays, a high content of MA generally increases the melt intercalation of PP chains in the clay structure which leads to a separation of the clay sheets, however, the presence of the MA can also generate im-miscibility with the PP matrix, thus affecting the me -chanical properties of the nanocomposites (Kato et al., 1997; Koo et al., 2003; Ville etal., 2012). The influence of the molecular weight is less clear; most authors have used low molecular weight MaPP (Kato et al., 1997; Kawasumi etal., 1997; Hasegawa etal., 1998; Hasegawa,
et al, 2000), nevertheless, high molecular weight impro-ves the mechanical properties. The presence of MaPP
El método de mezclado en fundido se utilizó para preparar materiales compuestos
termoplásticos reforzados con paligorskita; la modificación química de esta y el con -trol de los parámetros de extrusión se usaron para promover una buena dispersión y buena interface con la matriz polimérica, afectando las propiedades reológicas de la
mezcla, ya que el comportamiento viscoelástico en fundido es sensible a los cambios
en las estructuras moleculares tanto a nanoescala como a mesoescala. La nanoarcilla paligorskita se extrajo de una mina a cielo abierto situada en el sureste del estado de
Yucatán, México; esta arcilla fue sometida a un proceso de purificación y una modi
-ficación superficial con 3-aminopropiltrimetoxisilano. Estos procesos generaron tres tipos de especímenes: paligorskita sin purificar, purificada y purificada-silanizada;
las cuales fueron incorporadas (0.5 w%) a una matriz de polipropileno por extrusión de doble husillo. Barridos de frecuencia se emplearon para evaluar la interacción entre la matriz y el nano-refuerzo. Las curvas maestras del módulo de
almace-namiento (G’), módulo de pérdida (G”) y la viscosidad compleja (η*) vs la frecuencia angular (ωx) mostraron un cambio en la interacción interfacial polipropileno/ paligorskita cuando la arcilla se modificó químicamente.
• Paligorskita • morfología
• nanomateriales compuestos • reología
with different molecular weights not only affects the final morphology of the nanocomposite but also the melt behavior of the matrix (Reichert etal., 2000).
The size, shape, structure and surface characteristics of the disperse phase affect the rheological properties of the molten matrix, often negatively. However, with na-noparticles, the interaction between the reinforcement and the matrix takes place at the molecular level, di-rectly affecting molecular motion and flow. For this rea -son, the dispersion degree and interfacial interaction between nanoclay and a thermoplastic matrix affects the rheological properties of a nanocomposite, and knowledge of the nanocomposite rheological behavior leads to the optimization of the material processing (ex -trusion or injection).
A considerable number of studies have been con-ducted on the mechanical, rheological and thermal pro-perties of PSNs; Ghaffarpour and Khodaii (2009) found that by adding nanoclays to bitumen, the material’s rheological properties changed; not only the material stiffness increased, but also the phase angle (δ) decrea -sed and the aging resistance improved. Mahi and Ro-drigue (2012) performed dynamic rheological tests using ethylene vinyl acetate/nano-crystalline cellulose composites, at low frequencies, and a pseudo solid-like behavior was observed, which was correlated to parti-cle networks related to the hydrogen bonding between the cellulose molecules. Jin and Zhong (2013) perfor-med dynamic rheological tests to measure the storage (G ‘) and loss (G “) moduli at different temperatures using soy protein hydrogels reinforced with nanoclays to estimate the cross-linking time of the mixture. Little
information has been found related to the influence of nanoclay dispersion on the rheological properties of PSNs (Vaia etal., 1997). Hoffmann et al. (2000) and Lim and Park (2001) used rheological techniques to esta -blish that the linear viscoelastic properties of nanocom-posites are highly affected by the degree of clay dispersion at the polymeric matrix, particularly nano-composites where the polymer chains and the clay sur-face are chemically bonded (Krishnamoorti et al., 1996; Vaia & Giannelis, 1997). Some other factors should be considered to improve the properties of PSNs; as men-tioned by Murray and Zhou (2006), the amount of clay used and the physical properties of palygorskite and sepiolite like particle size, shape, distribution, surface area, chemical charge are a key factor to control the per-formance of the PSN’s, also due to the fibrillar nature of these clays, the fiber length is a parameter to be closely controlled to get high quality materials.
The clay used as reinforcement of the PSNs was palygorskite with an average diameter of 30 nm. Table 1 shows the chemical composition of the palygorskite (Soberanis G) extracted from a quarry located in Ticul, Yucatan, Mexico. The matrix used was isotactic polypro-pylene (PP). The compatibilizer was maleated polypro-pylene (MaPP); Table 2 shows the properties of the PP and MaPP. The palygorskite purification process utili -zed: hydrogen peroxide at 30% (w/v), glacial acetic
Table 1. Chemical composition of the extracted palygorskite measured by EDAX (Soberanis G)
Table 2. Physics properties of MaPP and PP
Material (g/10 min)MFI Mw Mn
(mg KOH/g) anhydride (%)Maleic Tm (°C)
Density (g/cm3) MaPP Aldrich 426512 115 107814 39417 5.34 0.5 152 0.95
acid, hydroxylamine chloride and sodium hexameta-phosphate, all of them reagent grade and hydrogen pe-roxide at 3.95% (w/v) medical grade. For the silanization process, 3-aminopropyltrimethoxysilane was used.
Extraction and purification of the palygorskite
The purification process of the palygorskite consisted of five treatments:
1) 30 g of palygorskite was mixed with 400 mL of disti-lled water for 3 h until total dispersion, after which the solution was filtered to remove stony debris.
2) 200 mL of hydrogen peroxide at 30% (w/v) was added and stirred until the bubbling ceased and then 300 mL of hydrogen peroxide at 3.95% (w/v) was added. Once the bubbling ended, the solution was heated at 100°C to evaporate the water; the addition of hydrogen peroxide at 3.95% (w/v) was repeated until no color change was observed in the solution. 3 mL of glacial acetic acid was added and the solution was evaporated; finally, the palygorskite was dried in an oven for 8 h at 100°C.
3) 240 mL of a solution 1 M of sodium acetate adjusted to pH 5 and 300 mL of distilled water were added to the palygorskite and stirred for 3 h. The mixture was then centrifuged at 1500 rpm for 15 min periods, and the sediments were decanted and dried in an oven at 100°C for 8 h.
4) 450 mL of hydroxylamine chloride 0.04 M and 150 mL of glacial acetic acid were added to the palygorskite and the mixture was heated at 96 ± 3°C with occasio-nal stirring for 6 h; 600 mL of distilled water was added to the palygorskite and stirred and evaporated for 30 min after which the mixture was centrifuged at 1500 rpm during 15 min periods; the palygorskite was washed until the liquid fraction was colorless and odorless; finally, the palygorskite was dried in an oven at 100°C for 8 h (Tessier et al., 1979).
5) 1000 mL of the dispersant solution of sodium hexa -metaphosphate at 0.5% (w/v) was added to the palygorskite and stirred for 8 h, after which the solu-tion was placed for 60 min in an ultrasonic bath, and centrifuged at 2000 rpm for 60 min; it was then de-canted and the palygorskite was dried in a vacuum oven at 80°C at -635 mm Hg. Finally, the palygorski -te was grinded and stored.
Silanization process of the purified palygorskite
Silanization of the palygorskite was performed using the following methodology: 500 mL of distilled water was added to 10 g of purified palygorskite and sonica -ted for 1 min; the solution was hea-ted to a temperature between 40 and 45°C and stirred for 10 min. 2.5 mL of 3-aminopropyltrimethoxysilane was added drop by drop for 60 min; the mixture was then centrifuged at 2000 rpm for 20 min and decanted. 25 mL of ethanol was added to each centrifuge tube and these were pla-ced in an ultrasonic bath for 10 min, after which 25 mL of distilled water was added to each tube and centrifu-ged at 2000 rpm for 10 min extra. 40 mL of distilled water was added to each centrifuge tube which were then sonicated for 10 min and centrifuged for 10 min at 2000 rpm. The solid material in the centrifuge tubes was dried in a vacuum oven at 80°C at -635 mm Hg. Finally, the palygorskite was grinded and stored.
3 mg of palygorskite were mixed with 130 mg of KBr and the mixture was subjected to a pressure of 10 ton in a Carver hydraulic press to mold a tablet that was dried in a vacuum oven at -635 mm Hg and 100ºC for 24 h. The spectrophotometer used was a Fourier Transform Infrared (FTIR) Nicolet model Protege 460. The spectra were obtained in the range from 4000 to 400 cm-1 with a
resolution of 4 cm-1 and 100 scans.
Scanning electron microscopy
Microscopic examination was performed to establish the morphology of the palygorskite before and after each one of the treatments from the purification pro -cess. The scanning electron microscope (SEM) used was a JEOL model JSM-6360-LV. The scans were performed with 20 kV in high vacuum mode with magnifications of 10,000x and 20,000x. The samples were coated with gold in a Denton Vacuum Desk-II cold sputtering ma -chine, with a deposition time of 18 s.
Extrusion and molding of the PSN’s
and 210°C, respectively. The extruder was fed with three dispensers calibrated to generate the formula: 0.5 wt% palygorskite, 10 wt% MaPP and 89.5 wt% PP. The extrudates were molded into sheets of 150 x 150 x 0.9 mm in a Carver semiautomatic press at 210°C with a progressive compression force of 4500 kgf.
Rheometric frequency sweeps
The rheological analysis was performed in a rheometer TA instrument, model AR-2000 fitted with parallel pla -tes of 25 mm of diameter. The frequency sweep experi -ments were performed on specimen disks with an average 25 mm diameter and 0.9 mm thickness; a pneu -matic pressure of 2.07 Bar and 10% strain was used, the test temperatures in the environmental chamber of the rheometer were 170, 190 and 210°C. Two methods were used for data acquisition:
1) Ascending frequency sweeps, where the frequency was increased from 0.1 to 200 rad/s at the three diffe -rent temperatures.
2) Descending frequency sweeps, where the frequen -cy was decreased from 200 to 0.1 rad/s at the three different temperatures (six frequency sweeps per sample).
Each frequency sweep was performed 2 min after the chamber reached the working temperature (170, 190, and 210°C) and the storage modulus (G’), loss modulus (G”) and complex viscosity (η*) vs angular frequency (ωx) were reported. The results of the six frequency sweeps from each sample and the principle of time-temperature superposition (TTS) were used to generate the master curves, which were calculated at a reference temperature of 170°C.
The time-temperature superposition principle was used to study the behavior of materials in a wide ran-ge of frequencies and/or temperatures. This principle transfers the information obtained to a single referen-ce temperature, thus it is possible to compare the re-sults from the different temperatures of all samples. The superposition principle is valid only when all re-laxation times aτ(T), in the Maxwell equation have the
same temperature dependence; mathematically, this principle can be expressed as (Morgan & Harris, 2004; Zhao et al., 2005; Ghaffarpour & Khodaii, 2009):
r = reference temperature
aτ = relation between two relaxation times at two
ρ(T) = density of the polymer at a temperature T
Results and discussion
Purification and silanization of the palygorskite
The purification of the palygorskite focused on the re -moval of stony waste and organic matter, and also pro -moted the ion exchange of calcium per sodium; the palygorskite collected from a mine naturally contains some contaminants which adversely affect the silaniza -tion process and therefore the compatibility with the thermoplastic matrix.
Figure 1 shows the FTIR spectra from the various steps of the palygorskite purification process. The ab -sorption bands at 3700–3200 cm−1 correspond to the
stretch vibrations of structural OH and OH of the bound and hygroscopic waters. The absorption band at 1700–1600 cm−1 is attributed to the bend vibration from
the hygroscopic, adsorbed and bound water or from structural OH. The bands between 1300 and 400 cm−1
are a combination of the stretch and bend vibrations of the Si or Al–O and octahedral M–OH (M represents me-tal element). Table 3 lists the band positions correspon-ding to the functional groups of the palygorskite (Madejová & Komadel, 2001; Cai et al., 2007; Cheng et al., 2011).
Figure 1. FTIR spectra of the different treatments from the palygorskite purification process
´( ,T ) ´( ,T)
G ω ρ G aτω
´´( ,T ) ´´( ,T)
G G aτ
The FTIR spectra from the different treatments of the purification process show no changes compared to the spectrum from untreated palygorskite. The only diffe -rences were observed at 1655 and 1635 cm-1, which
co-rrespond to water due to the hydrophilic nature of palygorskite. The spectrum from treatment 2 shows some difference at 1650 and 900 cm-1 which corresponds
to the bending vibration mode of the hygroscopic water and Si–O structures; however, subsequent treatments show no difference at all. The bands identified in Figure 1 are similar to those reported by Cai et al. in their FTIR study of palygorskite (2007), the palygorskite did not show any chemical damage related to the purification process.
Figure 2 compares the FTIR spectra of purified/silani -zed palygorskite and purified palygorskite. The spectrum of the clay after silanization with 3-aminopropyltrimeto -xysilane shows some differences in the regions correspon
-ding to the silane, which proves silane grafting to the palygorskite (after the silanization process, the palygors -kite was heavily washed with alcohol). Table 4 shows the band positions of the purified/silanized palygorskite (Madejová & Komadel, 2001).
The bands at 3212 cm-1 could be assigned to the
N—H stretching from the silane, the vibration at 1608 cm-1 also belongs to a silane amine group and it is
over-lapped with the 1628 cm-1 band characteristic of the
ab-sorbed water in the palygorskite; finally, the band at 1500 cm-1 corresponds to the absorption of an amino
group which is absent in the palygorskite spectrum. When the palygorskite reacted with the silane, the band intensity of 2930 cm-1 assigned to the C—H stretching
was increased due to the contribution from the organic portion of silane (Wang et al., 2014). In addition, the broad band at 3050 cm-1 corresponds to the vibrations
of the –NH3+ groups from the silane (Jag & Condrate,
1972; Rozenberg & Shoham, 2007).
Microscopy analysis of the palygorskite
SEM analysis was carried out on six different samples: palygorskite without treatment (as mined) and five palygorskite samples from each treatment of the purifi -cation process. Figure 3a clearly shows the fibrillar morphology of the palygorskite without treatment at 20,000x. Figures 3b to 3e show the treated nanofibers, their morphology, length and diameter seem to be simi-lar to the untreated fiber. However, Figure 3f shows na -nofibers with substantial length reduction; apparently, the last treatment of the purification process damaged the palygorskite, probably because this treatment in-volves a long period of centrifugation (60 min) and so-nication (60 min).
Table 3. FTIR band position for the palygorskite
Position (cm-1) Assignation
512 Octahedral deformation
484 Si-O (parallel to layer)
444 MgO6 (Rotation)
Table 4. FTIR bands from the purified/silanized palygorskite
Position (cm-1) Assignation
3615 Stretch Mg—OH dioctahedral
3516 Stretch OH of coordinated water with Al, Mg
3390 Stretch OH of zeolitic and absorbed water
3212 Stretch N—H
3050 Stretch N—H de amino (—NH3+)
2930 Stretch C—H
1625 Deformation OH of water
1500 Symmetric deformation N—H of amino (—NH
1470 Deformation C—H
Rheology analysis of the PP/MaPP/ Palygorskite for-mulations
The rheology properties of five different samples were measured: PP, a mixture of PP and MaPP and three for-mulations containing palygorskite with different che -mical treatments (Table 5).
The master curves of the PP frequency sweeps are shown in Figure 4; a long relaxation time τ = (1/ωx) =
(0.06868 ± 0.0045 s) was observed, corresponding to the frequency interval where the G’ and G” intersect (ωx =
14.56 ± 1.02 rad/s). Some frequency curves showed a small fluctuation of the data acquired at low frequen -cies; this was probably caused by the low torque signal which is near the resolution limit of the rheometer.
Figure 5 shows the rheological behavior of the mix -ture PP/MaPP; the relaxation time corresponding to the intersection of G’ and G” was ωx = 15.85 ± 0.39 rad/s is τ
= 0.06309 ± 0.0015 s. This intersection interval is shorter than that of PP. The loss modulus, storage modulus and complex viscosity at high frequencies of the mixtu
-re PP/MaPP a-re similar to those from PP (figu-re 4); which is to be expected since the mixture PP/MaPP con-tains only 10 wt% of MaPP (with 0.6% by weight of gra -fted maleic anhydride), therefore, the rheological behavior is dominated by the PP.
Based on the results from Table 6, it can be said that all the formulations initially showed a similar linear be-havior, since in all cases the G’, G” and η*, slopes are similar, but the frequency interval in which G’ and G” curve intersect is different for each formulation.
The rheological pattern of the PP/MaPP/UC formu -lation (Figure 6) is similar to PP, this could be caused by the low palygorskite content used (0.5 % by weight), as postulated by Zhao etal. (2005) “The number of parti -cles per unit volume is a key factor in establishing the characteristic rheological response of clay
nanocompo-Figure 3. SEM micrographs of the palygorskite without treatment and after the five treatments of the purification process, a) without treatment, b) treatment: 1. Distiller water, c) treatment:
2. Hydrogen peroxide, d) treatment:
3. Sodium acetate, e) treatment: 4. Hydroxylamine chloride, f) treatment: 5. Sodium
Table 5. Samples for the rheology test; the formulations were prepared by twin-screw extrusion
Formulation (wt%)PP (wt%)MaPP Palygorskite (wt%)
PP 100 0 0
PP/MaPP 90 10 0
UC 89.5 10 0.5 (Unpurified Clay)
PP/MaPP/PC 89.5 10 0.5 (Purified Clay)
PSC 89.5 10 0.5 (Purified and Silanized Clay)
sites”. In addition, the palygorskite used did not recei-ve any surface treatment, therefore, the palygorskite particles did not fully disperse, and consequently did not substantially contribute to the strengthening of the nanocomposite.
The rheological properties of the PP/MaPP/PC and PP/MaPP/PSC mixtures showed considerable diffe -rences when compared to PP. The PP/MaPP/PC (Figu-re 7) showed a dec(Figu-rease of G’, G” and η* both at high and low frequencies; this could be a result from the damage caused to the nanofibers of the palygorskite during the purification process (Figure 3) affecting their reinforcement ability due to the reduction of the fiber aspect ratio.
In contrast, PP/MaPP/PSC (Figure 8) showed a subs-tantial increase of G’, G” and η*, both at high and low frequency; although the fibers from the purified palygorskite had a reduced aspect ratio, the silaniza -tion process added func-tional groups to the fiber surfa -ce resulting in a better interfacial compatibility between
the matrix and the reinforcement. The amino groups grafted onto the surface of the palygorskite provided a chemical bond to the polymeric matrix; accordingly with Demjén etal. (1999), it is believed that during the extrusion process parcial thermal degradation of the PP/MaPP generates active carboxylic groups, which may chemically react with the amino groups of the gra-fted silane, providing covalent links between the palygorskite and the polymer matrix, and therefore, the relaxation time of the composite is increased.
Figure 9 shows the relaxation times from each sam-ple (Table 6); the relaxation times of the first three sam -ples show no substantial changes; however, the last two samples show a considerable change. PSNs with puri-fied palygorskite had a small relaxation time, conse -quently, the system became less elastic, resulting in a low matrix/reinforcement interaction, while the rein-forcing particles created areas of stress concentrations which affected the rheological properties; most likely caused by the damage suffered by the palygorskite du
-Figure 5. PP/MaPP master curve from the frequency sweeps: 0.1 to 200 and 200 to 0.1 rad/s at 170, 190 and 210°C. Reference temperature of 170°C
Table 6. Summary of the rheological properties from the five different samples studied
Properties PP PP/MaPPSAMPLEPP/MaPP/UC PP/MaPP/PC PP/MaPP/PSC
Wx (rad/s) 14.56±1.02 15.85±0.39 15.14±0.60 36.03±5.06 11.40±0.78
Slope Low freq.
G’ 1.17 1.17 1.22 1.28 1.18
G’’ 0.84 0.85 0.86 0.88 0.85
η* -0.15 -0.15 -0.12 -0.12 -0.14
G’ (Pa) 86340.37 81450.98 82969.69 51861.50 102606.69
G’’ (Pa) 49049.31 47776.72 48402.53 37018.50 54267.88
η* (Pa. S) 498.03 460.28 471.98 319.87 537.60
G’ (Pa) 40.19 41.37 30.34 14.54 49.55
G’’ (Pa) 308.76 301.99 254.37 144.89 335.81
η* (Pa. S) 12174.49 11488.99 10808.26 5337.88 14138.63
ring the purification process. The PSNs prepared with purified and silanized palygorskite became more elas -tic; this formulation reported the longest relaxation
time, which proves the existence of an interaction bet-ween matrix and reinforcement and therefore an im-provement of the rheological properties of PSNs.
The infrared spectrum of purified palygorskite is con -sistent with the spectrum of palygorskite reported in the literature. The palygorskite’s chemical structure was not affected by the extraction and purification pro -cesses.
The silanization method designed was able to che -mically attach the 3-aminopropyltrimethoxysilane to the nanofiber surface, as demonstrated by the infrared spectra. The presence of silane improved the interface between the palygorskite and the polypropylene, in-fluencing the rheological properties of the composite when melted.
SEM micrographs proved that the last treatment of the purification process, involving sodium hexameta -phosphate, centrifugation and sonication, caused a morphological change in the palygorskite: the aspect ratio was reduced.
The formulation PP/MaPP/PC prepared with puri-fied palygorskite reported the lowest values of storage modulus, probably caused by the low reinforcement content (0.5 wt%) and the damage caused to the palygorskite during the last treatment of the purifica -tion process. However, PSNs with purified/silanized palygorskite (PP/MaPP/PSC) improved their rheologi-cal properties compared to PP, despite the damage su-ffered by the palygorskite during the purification process.
Acknowledgment is given to Santiago Duarte Aranda for technical assistance on SEM analysis.
Abdul-Latif N. & Weaver C.E. Kinetic of acid-dissolution of palygorskite (attapulgite) and sepiolite. Clay and Clay Mine-rals, volume 17 (issue 3), January 1969: 169-178.
Bonilla J.L., López-González J. de D., Ramírez-Sáenz A., Ro
-dríguez-Reinoso F., Valenzuela-Calahorro C. Activation
of a sepiolite with dilute solutions of HNO3, and
subse-quent heat treatment: II. Determination of surface acid
centres. Clay Minerals, volume 16 (issue 2), September
Cai Y., Xue J., Polya D.A. A fourier transform infrared spectrosco-pic study of Mg-rich, Mg-poor and acid leached
palygorski-Figure 9. Relaxation times of the five formulations studied Figure 7. PP/MaPP/PC master curve from the frequency sweeps: 0.1 to 200 and 200 to 0.1 rad/s at 170, 190 y 210°C. Reference temperature of 170°C
tes, Spectrochimica Acta Part A. Molecular and Biomolecular Spectroscopy, volume 66 (issue 2), February 2007: 282-288.
Chen J., Jin Y., Qian Y., Hu T. A new approach to efficiently disper -se aggregated palygorskite into single crystal via adding
free-ze process into traditional extrusion treatment. IEEE Transaction on Nanotechnology, volume 9 (issue 1), January 2010: 6-10.
Cheng H., Yang J., Frost R.L., Wu Z. Infrared transmission and
emission spectroscopic study of selected chinese palygorski-tes. Part A. Spectrochimica Acta, volume 83 (issue 1), August
Corma A., Mifsud A., Sanz E. Influence of the chemical composi -tion and textural characteristics of palygorskite on the acid leaching of octahedral cations. Clay Minerals, volume 22 (issue
2), June 1987: 225-232.
Corma A., Mifsud A., Sanz E. Kinetics of the acid leaching of palygorskite; influence of the octahedral sheet composition. Clay Minerals, volume 25 (issue 2), June 1990: 197-205. Demjén Z., Pukánszky B., Nagy J. Possible coupling reactions of
functional silanes and polypropylene. Polymer, volume 40 (is-sue 7), March 1999: 1763-1773.
Dos Santos-Soares D., Santana-Fernandes C., S.Da Costa A.C.,
Nervo-Raffin F., Acchar W., De Lima-eMoura T.F.A. Charac
-terization of palygorskite clay from Piauí, Brazil and its po -tential use as excipient for solid dosage forms containing
anti-tuberculosis drugs. J. Therm Anal Calorim, volume 113
(issue 1), June 2013: 551-558.
Duan J., Shao S., Jiang L., Li y., Jing P., Liu B. Nano-attapulguite funcionalization by silane modification for preparation of co
-valently-integrated epoxy/TMPTMA nanocomposites. Iranian
Polymer Journal, volume 20 (issue 11), September 2011:
Furuichi N., Kurokawa Y., Fujita K., Oya A., Yasuda H., Kiso M. Preparation and properties of polypropylene reinforced by smectite. Journal of Materials Science, volume 31 (issue 16), Au-gust 1996: 4307-4310.
Ghaffarpour-Jahromi S. & Khodaii A. Effects of nanoclay on rheo -logical properties of bitumen binder. Construction and Building Materials, volume 23 (issue 8), March 2009: 2894-2904.
Gonzalez F., Pesquera C., Blanco C., Benito I., Mendioroz S., Paja -res J.A. Structural and textural evolution under thermal treatment of natural and acid-activated Al-rich and Mg-rich palygorskites. Applied Clay Science, volume 5 (issue 1), May
Hasegawa N., Kawasumi M., Kato M., Usuki A.,Okada A. Prepa-ration and mechanical properties of polypropylene-clay
hy-brids using a maleic anhydride-modified polypropylene
oligomer. Journal of Applied Polymer Science, volume 67 (issue 1), January 1998: 87-92.
Hasegawa N., Okamoto H., Kato M., Usuki A. Preparation and mechanical properties of polypropylene–clay hybrids based
on modified polypropylene and organophilic clay. Journal of
Applied Polymer Science, volume 78 (issue 11), December 2000: 1918-1922.
Hoffmann B., Dietrich C., Thomann R., Friedrich C., Mülhaupt R.
Morphology and rheology of polystyrene nanocomposites
based upon organoclay. Macromolecular Rapid
Communica-tions, volume 21 (issue 1), January 2000: 57-61.
Jang S.D. & Condrate R.A. The I.R. Spectra of Lysine Adsorbed on
Several Caution-Substituted Montmorillonites. Clay and Clay
Minerals, volume 20 (issue 2), April 1972: 79-82.
Jiménez-López A., López-González J. de D., Ramírez-Sáenz A., Rodríguez-Reinoso F., Valenzuela-Calahorro C., Zurita-He -rrera L. Evolution of surface area in a sepiolite as a function of acid and heat treatments. Clay Minerals, volume 13 (issue 4),
December 1978: 375-385.
Jin M. & Zhong Q. Transglutaminase cross-linking to enhance
elastic properties of soy protein hydrogels with intercalated montmorillonite nanoclay. Journal of Food Engineering, volume
115 (issue 1), March 2013: 33-40.
Kato M., Usuki A., Okada A. Synthesis of polypropylene oligo-mer-clay intercalation compounds. Journal of Applied Polymer Science, volume 66 (issue 9), November 1997: 1781-1785.
Kawasumi M., Hasegawa N., Kato M., Usuki A., Okada A. Prepa-ration and mechanical properties of polypropylene-clay
hy-brids. Macromolecules, volume 30 (issue 20), October 1997:
Kojima Y., Usuki A., Kawasumi M., Okada A., Fukushima Y., Ku-rauchi T., Kamigaito O. Mechanical properties of nylon 6-clay hybrid. Journal of Materials Research, volume 8 (issue 5), May 1993: 1185-1189.
Koo C.M., Kim J.H., Wang K.H., Chung I.J. Melt-Extensional Pro -perties and Orientation Behaviors of Polypropylene-Layered Silicate Nanocomposites. Journal of Polymer Science: Part B:
Po-lymer Physics, volume 43 (issue 2), January 2005: 158-167.
Koo C.M., Kim M.J., Choi M.H., Kim S.O., Chung I.J. Mechanical and rheological properties of the maleated
polypropylene–la-yered silicate nanocomposites with different morphology. Journal of Applied Polymer Science, volume 88 (issue 6), May
Krishnamoorti R., Vaia R.A., Giannelis E.P. Structure and
Dy-namics of Polymer-Layered Silicate Nanocomposites.
Che-mistry of Materials, volume 8 (issue 8), August 1996: 1728-1734.
Lim Y.T. & Park O.O. Phase morphology and rheological behavior
of polymer/layered silicate nanocomposites. Rheologica Acta, volume 40 (issue 3), May 2001: 220-229.
Madejová J. & Komadel P. Baseline of the Clay Minerals Society
Source Clays: Infrared Methods. Clays and Clay Minerals,
volu-me 49 (issue 5), October 2001: 410-432.
Mahi H. & Rodrigue D. Linear and non-linear viscoelastic proper -ties of ethylene vinyl acetate/nano-crystalline cellulose com-posites. Rheologica Acta, volume 51 (issue 2), February 2012:
Morgan A.B. & Harris J.D. Exfoliated polystyrene-clay nanocom
-posites synthesized by solvent blending with sonication. Poly-mer, volume 45 (issue 26), December 2004: 8695-8703. Murray H.H. & Zhou H. Palygorskite and Sepiolite (Hormites) en:
Kogel J.E., Trivedi N.C., Barker J.M., Krukowski S.T. Industrial Minerals and Rocks, 7th ed., New York,Society for Mining,
Me-tallurgy, and Exploration, 2006, chapter 23, pp. 401-406.
Pesquera C., González F., Benito I., Blanco C., Mendioroz S., Paja -res J.A. Passivation of a montmorillonite by the silica created in acid activation. Journal of Materials Chemistry, volume 2 (is-sue 9), September 1992: 907-911.
Reichert P., Nitz H., Klinke S., Brandsch R., Thomann R., Mülhaupt
R. Poly (propylene)/organoclay nanocomposite formation:
In-fluence of compatibilizer functionality and organoclay modi
-fication. Macromolecular Materials and Engineering, volume 275
(issue 1), February 2000: 8-17.
Rozenberg M. & Shoham G. FTIR spectra of solid poly-l-lysine in
the stretching NH mode range. Biophysical Chemistry, volume
125 (issue 1), January 2007: 166-171.
Soberanis G. Propiedades reológicas en fundido de materiales compues-tos termoplásticos reforzados con nanoarcilla de paligorskita, (tesis doctorado en ciencia), Mérida Yucatán, Centro de
Investiga-ción Científica de Yucatán, 2015, 156 pp.
Tessier A., Campbell P.G.C. & Bisson M. Sequential extraction
procedure for the speciation of particulate trace metals.
Analytical Chemistry, volume 51 (issue 7), June 1979: 844-851.
Vaia R.A., Sauer B.B., Tse O.K., Giannelis E.P. Relaxations of
con-fined chains in polymer nanocomposites: Glass transition pro -perties of poly (ethylene oxide) intercalated in montmorillonite. Journal of Polymer Science, Part B: Polymer
Physics, volume 35 (issue 1), January 1997: 59-67.
Vaia R.A. & Giannelis E.P. Polymer Melt Intercalation in Organi
-cally-Modified Layered Silicates: Model Predictions and Ex
-periment. Macromolecules, volume 30 (issue 25), December
Ville J., Médéric P., Huitric J., Aubry T. Structural and rheological investigation of interphase in polyethylene/polyamide/nano-clay ternary blends. Polymer, volume 53 (issue 8), February
Wang K.H., Xu M., Choi Y.S., Chung I.J. Effect of aspect ratio of
clay on melt extensional process of maleated polyethylene/ clay nanocomposites. Polymer Bulletin, volume 46 (issue 6),
July 2001: 499-505.
Wang C., Ding L., Wu Q., Liu F., Wei J., Lu R., Xie H., Cheng R. Soy polyol-based polyurethane modified by raw silylated
palygorskite. Industrial Crops and Products, volume 57 (issue
1), March 2014: 29-34.
Zhao J., Morgan A.B., Harris J.D. Rheological characterization of
polystyrene–clay nanocomposites to compare the degree of exfoliation and dispersion. Polymer, volume 46 (issue 20),
September 2005: 8641-8660.
Citation for this article: Chicago citation style
Soberanis-Monforte, Genaro Antonio, José Luis Gordillo-Rubio, Pedro Iván González-Chi. Influence of chemically treated palygors-kite over the rheological behavior of polypropylene nanocomposi-tes. Ingeniería Investigación y Tecnología, XVI, 04 (2015): 491-501.
ISO 690 citation style
Soberanis-Monforte G.A., Gordillo-Rubio J.L., González-Chi P.I. Influence of chemically treated palygorskite over the rheological behavior of polypropylene nanocomposites. Ingeniería Investiga-ción y Tecnología, volume XVI (issue 4), October-December 2015: 491-501.
About the authors
Genaro Antonio Soberanis-Monforte. PhD student on science of polymeric materials from Centro de Investigación
Científica de Yucatán, A.C., master degree on polymeric materials from Centro de Investigación Científica de Yucatán, A.C., mechanical engineering from Instituto Tecnológico de Mérida. Certified engineer on
leakage tests by PEMEX gas station franchise, Lechurer of the Universidad Tecnológica Metropolitana, of the Universidad Marista de Mérida and the Universidad Autónoma de Yucatán.
Pedro Iván González-Chi. PhD on polymer science and technology from Manchester Materials Science Centre/ UMIST. MSc. on polymer science and technology from Manchester Materials Science Centre/UMIST.
In-dustrial chemical engineering from Universidad Autónoma de Yucatán. Working experience: 1998 to 2000: associate researcher, Centro de Investigación Científica de Yucatán, A.C., 2001 to date, titular researcher. Centro de Investigación Científica de Yucatán, A.C., 2009 to date, Head of the Materials Department. Cen
-tro de Investigación Científica de Yucatán, A.C.
José Luis Gordillo-Rubio, Industrial chemist from the Chemical Engineering School of the Universidad